#------------------------------------------------------------------------------
#$Date: 2016-03-22 11:51:51 +0200 (Tue, 22 Mar 2016) $
#$Revision: 178920 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/49/4114915.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4114915
loop_
_publ_author_name
'Xiqu Wang'
'Lumei Liu'
'Allan J. Jacobson'
_publ_contact_author_address
;
Department of Chemistry    
University of Houston,
Houston, TX 77204-5003
;
_publ_contact_author_email       ' ajjcob@uh.edu '
_publ_contact_author_fax         ' 713 743 2787 '
_publ_contact_author_name
;
Prof. Allan J. Jacobson
;
_publ_contact_author_phone       ' 713 743 2785 '
_publ_section_title
;
 Open-Framework and Microporous Vanadium Silicates
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              7812
_journal_page_last               7820
_journal_paper_doi               10.1021/ja020354l
_journal_volume                  124
_journal_year                    2002
_chemical_formula_sum            'H6 O14 Rb2 Si4 V'
_chemical_formula_weight         564.29
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_atom_sites_solution_hydrogens   IGNORED
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   13.1698(6)
_cell_length_b                   13.1698(6)
_cell_length_c                   14.5054(8)
_cell_measurement_temperature    293(2)
_cell_volume                     2178.81(18)
_computing_cell_refinement       SAINT
_computing_data_collection       SMART
_computing_data_reduction        SAINT
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    SHELXTL
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.977
_diffrn_measured_fraction_theta_max 0.977
_diffrn_measurement_device_type  'SIEMENS SMART/CCD'
_diffrn_measurement_method       'NARROW FRAME, 0.3w'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0476
_diffrn_reflns_av_sigmaI/netI    0.0183
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            12999
_diffrn_reflns_theta_full        28.30
_diffrn_reflns_theta_max         28.30
_diffrn_reflns_theta_min         1.79
_exptl_absorpt_coefficient_mu    7.738
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.4820
_exptl_absorpt_correction_type   'multi-scan (SADABS)'
_exptl_crystal_colour            BLUE-GREEN
_exptl_crystal_density_diffrn    2.580
_exptl_crystal_description       PRISM
_exptl_crystal_F_000             1626
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.05
_refine_diff_density_max         2.317
_refine_diff_density_min         -0.856
_refine_diff_density_rms         0.225
_refine_ls_extinction_coef       0.0035(10)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.099
_refine_ls_hydrogen_treatment    NA
_refine_ls_matrix_type           full
_refine_ls_number_parameters     106
_refine_ls_number_reflns         1039
_refine_ls_number_restraints     4
_refine_ls_restrained_S_all      1.122
_refine_ls_R_factor_all          0.0938
_refine_ls_R_factor_gt           0.0791
_refine_ls_shift/su_max          0.894
_refine_ls_shift/su_mean         0.015
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1634P)²+11.2786P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2442
_refine_ls_wR_factor_ref         0.2581
_reflns_number_gt                828
_reflns_number_total             1039
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja020354l_06.cif
_cod_data_source_block           VSH-6Rb
_cod_database_code               4114915
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-y, -x, -z+1/2'
'-x+y, y, -z+1/2'
'x, x-y, -z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z-1/2'
'x-y, -y, z-1/2'
'-x, -x+y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Rb1 Rb 0.5000 0.5000 0.5000 0.0691(8) Uani 1 4 d S
Rb2 Rb 0.3017(3) 0.15084(13) 0.38351(16) 0.0547(8) Uani 0.50 2 d SP
V1 V 0.1906(2) 0.3812(4) 0.4592(3) 0.0118(10) Uani 0.25 2 d SPD
V2 V 0.1584(5) 0.3168(10) 0.4353(6) 0.048(2) Uani 0.25 2 d SPD
Si1 Si 0.32809(17) 0.43396(16) 0.2500 0.0236(6) Uani 1 2 d SD
Si2 Si -0.0064(2) 0.2296(2) 0.37671(19) 0.0160(7) Uani 0.50 1 d P
O1 O 0.4593(3) 0.5407(3) 0.2500 0.032(2) Uani 1 4 d S
O2 O 0.2376(4) 0.4752(9) 0.2791(7) 0.019(2) Uani 0.50 2 d SP
O3 O 0.2981(8) 0.3868(11) 0.3607(6) 0.045(3) Uani 0.50 1 d PD
O4 O 0.3220(7) 0.3330(7) 0.3065(6) 0.037(2) Uani 0.50 1 d PD
O5 O 0.1100(7) 0.2200(13) 0.3800(12) 0.033(3) Uani 0.50 2 d SP
O6 O -0.0432(8) 0.2518(8) 0.4766(6) 0.037(2) Uani 0.50 1 d P
O7 O 0.2189(11) 0.1095(5) 0.3296(7) 0.025(2) Uani 0.50 2 d SP
O8 O 0.2573(7) 0.5145(13) 0.4883(13) 0.017(4) Uiso 0.25 2 d SPD
O9 O 0.110(3) 0.220(7) 0.351(5) 0.16(4) Uiso 0.25 2 d SPD
OW1 O 0.0000 0.0000 0.2500 0.13(3) Uani 0.50 12 d SP
OW2 O 0.524(9) 0.262(4) 0.2500 0.4(2) Uani 0.17 4 d SP
OW3 O 0.583(2) 0.417(2) 0.345(4) 0.094(19) Uani 0.20 2 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
OW3 Rb1 OW3 180.000(2) . 13_666
OW3 Rb1 O6 100.92(19) . 8_666
OW3 Rb1 O6 79.08(19) 13_666 8_666
OW3 Rb1 O6 79.08(19) . 2_665
OW3 Rb1 O6 100.92(19) 13_666 2_665
O6 Rb1 O6 22.7(4) 8_666 2_665
OW3 Rb1 O6 79.08(19) . 20
OW3 Rb1 O6 100.92(19) 13_666 20
O6 Rb1 O6 180.0 8_666 20
O6 Rb1 O6 157.3(4) 2_665 20
OW3 Rb1 O6 100.92(19) . 14_556
OW3 Rb1 O6 79.08(19) 13_666 14_556
O6 Rb1 O6 157.3(4) 8_666 14_556
O6 Rb1 O6 180.0 2_665 14_556
O6 Rb1 O6 22.7(4) 20 14_556
OW3 Rb1 O3 106.9(6) . 13_666
OW3 Rb1 O3 73.1(7) 13_666 13_666
O6 Rb1 O3 46.9(2) 8_666 13_666
O6 Rb1 O3 50.0(2) 2_665 13_666
O6 Rb1 O3 133.1(2) 20 13_666
O6 Rb1 O3 130.0(2) 14_556 13_666
OW3 Rb1 O3 73.1(6) . .
OW3 Rb1 O3 106.9(7) 13_666 .
O6 Rb1 O3 133.1(2) 8_666 .
O6 Rb1 O3 130.0(2) 2_665 .
O6 Rb1 O3 46.9(2) 20 .
O6 Rb1 O3 50.0(2) 14_556 .
O3 Rb1 O3 180.000(1) 13_666 .
OW3 Rb1 O3 73.1(6) . 19_665
OW3 Rb1 O3 106.9(6) 13_666 19_665
O6 Rb1 O3 50.0(2) 8_666 19_665
O6 Rb1 O3 46.9(2) 2_665 19_665
O6 Rb1 O3 130.0(2) 20 19_665
O6 Rb1 O3 133.1(2) 14_556 19_665
O3 Rb1 O3 94.9(4) 13_666 19_665
O3 Rb1 O3 85.1(4) . 19_665
OW3 Rb1 O3 106.9(6) . 7_556
OW3 Rb1 O3 73.1(6) 13_666 7_556
O6 Rb1 O3 130.0(2) 8_666 7_556
O6 Rb1 O3 133.1(2) 2_665 7_556
O6 Rb1 O3 50.0(2) 20 7_556
O6 Rb1 O3 46.9(2) 14_556 7_556
O3 Rb1 O3 85.1(4) 13_666 7_556
O3 Rb1 O3 94.9(4) . 7_556
O3 Rb1 O3 180.000(1) 19_665 7_556
OW3 Rb1 O8 57.8(8) . 13_666
OW3 Rb1 O8 122.2(8) 13_666 13_666
O6 Rb1 O8 72.1(3) 8_666 13_666
O6 Rb1 O8 54.2(3) 2_665 13_666
O6 Rb1 O8 107.9(3) 20 13_666
O6 Rb1 O8 125.8(3) 14_556 13_666
O3 Rb1 O8 50.6(3) 13_666 13_666
O3 Rb1 O8 129.4(3) . 13_666
O3 Rb1 O8 91.1(4) 19_665 13_666
O3 Rb1 O8 88.9(4) 7_556 13_666
OW3 Rb1 O8 122.2(8) . .
OW3 Rb1 O8 57.8(8) 13_666 .
O6 Rb1 O8 107.9(3) 8_666 .
O6 Rb1 O8 125.8(3) 2_665 .
O6 Rb1 O8 72.1(3) 20 .
O6 Rb1 O8 54.2(3) 14_556 .
O3 Rb1 O8 129.4(3) 13_666 .
O3 Rb1 O8 50.6(3) . .
O3 Rb1 O8 88.9(4) 19_665 .
O3 Rb1 O8 91.1(4) 7_556 .
O8 Rb1 O8 180.000(2) 13_666 .
O7 Rb2 Si2 67.21(19) . 3
O7 Rb2 Si2 67.21(19) . 20
Si2 Rb2 Si2 125.6(2) 3 20
O7 Rb2 O6 114.6(4) . 3
Si2 Rb2 O6 52.4(3) 3 3
Si2 Rb2 O6 131.1(3) 20 3
O7 Rb2 O6 114.6(4) . 20
Si2 Rb2 O6 131.1(3) 3 20
Si2 Rb2 O6 52.4(3) 20 20
O6 Rb2 O6 90.9(5) 3 20
O7 Rb2 V1 151.3(6) . 14_556
Si2 Rb2 V1 102.88(14) 3 14_556
Si2 Rb2 V1 102.88(14) 20 14_556
O6 Rb2 V1 50.5(3) 3 14_556
O6 Rb2 V1 50.5(3) 20 14_556
O7 Rb2 O4 77.8(3) . 21
Si2 Rb2 O4 38.8(2) 3 21
Si2 Rb2 O4 144.0(3) 20 21
O6 Rb2 O4 71.1(3) 3 21
O6 Rb2 O4 161.5(3) 20 21
V1 Rb2 O4 112.1(2) 14_556 21
O7 Rb2 O4 77.8(3) . .
Si2 Rb2 O4 144.0(3) 3 .
Si2 Rb2 O4 38.8(2) 20 .
O6 Rb2 O4 161.5(3) 3 .
O6 Rb2 O4 71.1(3) 20 .
V1 Rb2 O4 112.1(2) 14_556 .
O4 Rb2 O4 126.5(4) 21 .
O7 Rb2 V2 133.4(6) . 14_556
Si2 Rb2 V2 95.12(17) 3 14_556
Si2 Rb2 V2 95.12(17) 20 14_556
O6 Rb2 V2 45.8(2) 3 14_556
O6 Rb2 V2 45.8(2) 20 14_556
V1 Rb2 V2 17.9(2) 14_556 14_556
O4 Rb2 V2 115.7(2) 21 14_556
O4 Rb2 V2 115.7(2) . 14_556
O7 Rb2 O8 177.8(6) . 14_556
Si2 Rb2 O8 113.34(15) 3 14_556
Si2 Rb2 O8 113.34(15) 20 14_556
O6 Rb2 O8 66.7(4) 3 14_556
O6 Rb2 O8 66.7(3) 20 14_556
V1 Rb2 O8 30.9(3) 14_556 14_556
O4 Rb2 O8 101.3(3) 21 14_556
O4 Rb2 O8 101.3(3) . 14_556
V2 Rb2 O8 48.8(4) 14_556 14_556
O7 Rb2 O6 106.2(4) . 7_556
Si2 Rb2 O6 46.32(18) 3 7_556
Si2 Rb2 O6 127.0(2) 20 7_556
O6 Rb2 O6 8.7(3) 3 7_556
O6 Rb2 O6 92.7(2) 20 7_556
V1 Rb2 O6 56.88(17) 14_556 7_556
O4 Rb2 O6 70.1(3) 21 7_556
O4 Rb2 O6 163.2(3) . 7_556
V2 Rb2 O6 49.60(17) 14_556 7_556
O8 Rb2 O6 75.2(3) 14_556 7_556
O7 Rb2 O6 106.2(4) . 14_556
Si2 Rb2 O6 127.0(2) 3 14_556
Si2 Rb2 O6 46.32(18) 20 14_556
O6 Rb2 O6 92.7(2) 3 14_556
O6 Rb2 O6 8.7(3) 20 14_556
V1 Rb2 O6 56.88(17) 14_556 14_556
O4 Rb2 O6 163.2(3) 21 14_556
O4 Rb2 O6 70.1(3) . 14_556
V2 Rb2 O6 49.60(17) 14_556 14_556
O8 Rb2 O6 75.2(3) 14_556 14_556
O6 Rb2 O6 93.2(3) 7_556 14_556
V2 V1 O8 170.2(10) . .
V2 V1 O6 75.3(6) . 9_556
O8 V1 O6 111.2(6) . 9_556
V2 V1 O6 75.3(6) . 14_556
O8 V1 O6 111.2(6) . 14_556
O6 V1 O6 90.8(5) 9_556 14_556
V2 V1 O3 73.8(6) . 20
O8 V1 O3 99.3(6) . 20
O6 V1 O3 82.5(4) 9_556 20
O6 V1 O3 149.1(5) 14_556 20
V2 V1 O3 73.8(6) . .
O8 V1 O3 99.3(6) . .
O6 V1 O3 149.1(5) 9_556 .
O6 V1 O3 82.5(4) 14_556 .
O3 V1 O3 87.9(5) 20 .
V2 V1 O5 6.7(7) . .
O8 V1 O5 163.5(9) . .
O6 V1 O5 79.8(5) 9_556 .
O6 V1 O5 79.8(5) 14_556 .
O3 V1 O5 69.3(5) 20 .
O3 V1 O5 69.3(5) . .
V2 V1 O9 15(2) . .
O8 V1 O9 155(3) . .
O6 V1 O9 85.7(17) 9_556 .
O6 V1 O9 85.6(17) 14_556 .
O3 V1 O9 63.9(16) 20 .
O3 V1 O9 63.8(16) . .
O5 V1 O9 8(3) . .
V2 V1 Rb2 93.6(7) . 15_556
O8 V1 Rb2 96.2(7) . 15_556
O6 V1 Rb2 50.5(3) 9_556 15_556
O6 V1 Rb2 50.5(3) 14_556 15_556
O3 V1 Rb2 132.9(3) 20 15_556
O3 V1 Rb2 132.9(3) . 15_556
O5 V1 Rb2 100.3(5) . 15_556
O9 V1 Rb2 109(2) . 15_556
V2 V1 Si2 38.20(16) . .
O8 V1 Si2 138.8(3) . .
O6 V1 Si2 56.9(3) 9_556 .
O6 V1 Si2 108.4(4) 14_556 .
O3 V1 Si2 43.6(4) 20 .
O3 V1 Si2 96.6(4) . .
O5 V1 Si2 37.28(9) . .
O9 V1 Si2 37.6(3) . .
Rb2 V1 Si2 100.32(17) 15_556 .
V2 V1 Si2 38.20(16) . 20
O8 V1 Si2 138.8(3) . 20
O6 V1 Si2 108.4(4) 9_556 20
O6 V1 Si2 56.9(3) 14_556 20
O3 V1 Si2 96.6(4) 20 20
O3 V1 Si2 43.6(4) . 20
O5 V1 Si2 37.29(9) . 20
O9 V1 Si2 37.5(3) . 20
Rb2 V1 Si2 100.32(17) 15_556 20
Si2 V1 Si2 74.40(18) . 20
V2 V1 Rb1 114.17(8) . 3_565
O8 V1 Rb1 66.07(9) . 3_565
O6 V1 Rb1 57.5(3) 9_556 3_565
O6 V1 Rb1 139.6(3) 14_556 3_565
O3 V1 Rb1 58.2(3) 20 3_565
O3 V1 Rb1 137.6(3) . 3_565
O5 V1 Rb1 113.90(8) . 3_565
O9 V1 Rb1 113.2(3) . 3_565
Rb2 V1 Rb1 89.21(10) 15_556 3_565
Si2 V1 Rb1 76.62(6) . 3_565
Si2 V1 Rb1 150.67(16) 20 3_565
V1 V2 O5 169.3(11) . .
V1 V2 O9 158(4) . .
O5 V2 O9 12(4) . .
V1 V2 O6 80.2(6) . 14_556
O5 V2 O6 106.9(7) . 14_556
O9 V2 O6 114(2) . 14_556
V1 V2 O6 80.2(6) . 9_556
O5 V2 O6 106.9(7) . 9_556
O9 V2 O6 114(2) . 9_556
O6 V2 O6 93.1(6) 14_556 9_556
V1 V2 O3 82.3(7) . .
O5 V2 O3 90.3(7) . .
O9 V2 O3 82(2) . .
O6 V2 O3 85.1(4) 14_556 .
O6 V2 O3 162.4(9) 9_556 .
V1 V2 O3 82.3(7) . 20
O5 V2 O3 90.3(7) . 20
O9 V2 O3 82(2) . 20
O6 V2 O3 162.4(9) 14_556 20
O6 V2 O3 85.1(4) 9_556 20
O3 V2 O3 91.4(6) . 20
V1 V2 Si2 127.7(3) . .
O5 V2 Si2 50.8(3) . .
O9 V2 Si2 51.1(4) . .
O6 V2 Si2 140.9(6) 14_556 .
O6 V2 Si2 69.7(3) 9_556 .
O3 V2 Si2 121.5(5) . .
O3 V2 Si2 54.2(4) 20 .
V1 V2 Si2 127.7(3) . 20
O5 V2 Si2 50.8(3) . 20
O9 V2 Si2 51.0(4) . 20
O6 V2 Si2 69.7(3) 14_556 20
O6 V2 Si2 140.9(6) 9_556 20
O3 V2 Si2 54.2(4) . 20
O3 V2 Si2 121.5(5) 20 20
Si2 V2 Si2 101.3(5) . 20
V1 V2 O8 6.5(7) . .
O5 V2 O8 162.9(9) . .
O9 V2 O8 151(4) . .
O6 V2 O8 84.6(6) 14_556 .
O6 V2 O8 84.6(6) 9_556 .
O3 V2 O8 77.8(6) . .
O3 V2 O8 77.8(6) 20 .
Si2 V2 O8 126.1(3) . .
Si2 V2 O8 126.1(3) 20 .
V1 V2 O6 99.8(4) . .
O5 V2 O6 84.1(5) . .
O9 V2 O6 88.8(14) . .
O6 V2 O6 117.4(4) 14_556 .
O6 V2 O6 29.0(5) 9_556 .
O3 V2 O6 157.5(5) . .
O3 V2 O6 66.9(4) 20 .
Si2 V2 O6 40.8(2) . .
Si2 V2 O6 131.7(6) 20 .
O8 V2 O6 102.1(4) . .
V1 V2 O6 99.8(4) . 20
O5 V2 O6 84.1(5) . 20
O9 V2 O6 88.6(14) . 20
O6 V2 O6 29.0(5) 14_556 20
O6 V2 O6 117.4(4) 9_556 20
O3 V2 O6 66.9(4) . 20
O3 V2 O6 157.5(5) 20 20
Si2 V2 O6 131.7(6) . 20
Si2 V2 O6 40.8(2) 20 20
O8 V2 O6 102.1(4) . 20
O6 V2 O6 133.6(6) . 20
O4 Si1 O4 64.8(7) 16_556 .
O4 Si1 O1 109.3(4) 16_556 .
O4 Si1 O1 109.3(4) . .
O4 Si1 O2 115.6(5) 16_556 16_556
O4 Si1 O2 135.6(5) . 16_556
O1 Si1 O2 111.5(4) . 16_556
O4 Si1 O2 135.6(5) 16_556 .
O4 Si1 O2 115.6(5) . .
O1 Si1 O2 111.5(4) . .
O2 Si1 O2 30.7(7) 16_556 .
O4 Si1 O3 43.4(5) 16_556 16_556
O4 Si1 O3 106.7(6) . 16_556
O1 Si1 O3 105.9(4) . 16_556
O2 Si1 O3 78.3(5) 16_556 16_556
O2 Si1 O3 107.4(5) . 16_556
O4 Si1 O3 106.7(6) 16_556 .
O4 Si1 O3 43.4(5) . .
O1 Si1 O3 105.9(4) . .
O2 Si1 O3 107.4(5) 16_556 .
O2 Si1 O3 78.3(5) . .
O3 Si1 O3 142.6(9) 16_556 .
O4 Si1 Rb2 4.2(4) 16_556 16_556
O4 Si1 Rb2 60.9(4) . 16_556
O1 Si1 Rb2 111.6(3) . 16_556
O2 Si1 Rb2 116.8(4) 16_556 16_556
O2 Si1 Rb2 134.7(3) . 16_556
O3 Si1 Rb2 46.7(4) 16_556 16_556
O3 Si1 Rb2 102.6(4) . 16_556
O4 Si1 Rb2 60.9(4) 16_556 .
O4 Si1 Rb2 4.2(4) . .
O1 Si1 Rb2 111.6(3) . .
O2 Si1 Rb2 134.7(3) 16_556 .
O2 Si1 Rb2 116.8(4) . .
O3 Si1 Rb2 102.6(4) 16_556 .
O3 Si1 Rb2 46.7(4) . .
Rb2 Si1 Rb2 56.99(6) 16_556 .
O4 Si1 Rb1 116.0(3) 16_556 .
O4 Si1 Rb1 59.9(4) . .
O1 Si1 Rb1 64.87(7) . .
O2 Si1 Rb1 125.8(3) 16_556 .
O2 Si1 Rb1 96.9(3) . .
O3 Si1 Rb1 155.7(3) 16_556 .
O3 Si1 Rb1 41.3(4) . .
Rb2 Si1 Rb1 113.48(5) 16_556 .
Rb2 Si1 Rb1 63.95(4) . .
O4 Si1 Rb1 59.9(4) 16_556 4_664
O4 Si1 Rb1 116.0(3) . 4_664
O1 Si1 Rb1 64.87(7) . 4_664
O2 Si1 Rb1 96.9(3) 16_556 4_664
O2 Si1 Rb1 125.8(3) . 4_664
O3 Si1 Rb1 41.3(4) 16_556 4_664
O3 Si1 Rb1 155.7(3) . 4_664
Rb2 Si1 Rb1 63.95(4) 16_556 4_664
Rb2 Si1 Rb1 113.48(5) . 4_664
Rb1 Si1 Rb1 122.78(5) . 4_664
O6 Si2 O5 112.1(7) . .
O6 Si2 O4 110.1(5) . 20
O5 Si2 O4 110.2(6) . 20
O6 Si2 O7 112.0(5) . 2
O5 Si2 O7 107.5(7) . 2
O4 Si2 O7 104.5(5) 20 2
O6 Si2 O9 127(2) . .
O5 Si2 O9 15(3) . .
O4 Si2 O9 100(4) 20 .
O7 Si2 O9 100.7(15) 2 .
O6 Si2 Rb2 72.7(3) . 2
O5 Si2 Rb2 142.8(6) . 2
O4 Si2 Rb2 101.5(3) 20 2
O7 Si2 Rb2 43.8(4) 2 2
O9 Si2 Rb2 142(2) . 2
O6 Si2 O3 90.4(5) . 20
O5 Si2 O3 87.2(6) . 20
O4 Si2 O3 40.3(4) 20 20
O7 Si2 O3 144.5(5) 2 20
O9 Si2 O3 86(3) . 20
Rb2 Si2 O3 130.0(3) 2 20
O6 Si2 V2 81.7(4) . .
O5 Si2 V2 41.3(6) . .
O4 Si2 V2 97.1(4) 20 .
O7 Si2 V2 147.7(5) 2 .
O9 Si2 V2 51.2(7) . .
Rb2 Si2 V2 152.3(3) 2 .
O3 Si2 V2 59.0(4) 20 .
O6 Si2 O6 30.3(5) . 9_556
O5 Si2 O6 84.0(7) . 9_556
O4 Si2 O6 112.2(4) 20 9_556
O7 Si2 O6 134.7(4) 2 9_556
O9 Si2 O6 97.9(15) . 9_556
Rb2 Si2 O6 101.9(3) 2 9_556
O3 Si2 O6 77.5(4) 20 9_556
V2 Si2 O6 51.6(3) . 9_556
O6 Si2 V1 74.0(3) . .
O5 Si2 V1 55.1(6) . .
O4 Si2 V1 88.7(3) 20 .
O7 Si2 V1 161.7(5) 2 .
O9 Si2 V1 63.8(10) . .
Rb2 Si2 V1 146.6(2) 2 .
O3 Si2 V1 48.8(3) 20 .
V2 Si2 V1 14.1(3) . .
O6 Si2 V1 45.5(2) 9_556 .
O6 Si2 Rb2 47.4(4) . 15_556
O5 Si2 Rb2 65.2(6) . 15_556
O4 Si2 Rb2 121.2(3) 20 15_556
O7 Si2 Rb2 133.6(4) 2 15_556
O9 Si2 Rb2 79.5(18) . 15_556
Rb2 Si2 Rb2 113.74(14) 2 15_556
O3 Si2 Rb2 81.8(3) 20 15_556
V2 Si2 Rb2 38.52(19) . 15_556
O6 Si2 Rb2 19.3(2) 9_556 15_556
V1 Si2 Rb2 38.10(12) . 15_556
O6 Si2 Rb1 45.3(4) . 3_565
O5 Si2 Rb1 117.9(6) . 3_565
O4 Si2 Rb1 66.2(3) 20 3_565
O7 Si2 Rb1 134.1(4) 2 3_565
O9 Si2 Rb1 125.0(17) . 3_565
Rb2 Si2 Rb1 92.17(13) 2 3_565
O3 Si2 Rb1 48.7(3) 20 3_565
V2 Si2 Rb1 76.7(3) . 3_565
O6 Si2 Rb1 50.2(2) 9_556 3_565
V1 Si2 Rb1 62.79(9) . 3_565
Rb2 Si2 Rb1 66.96(5) 15_556 3_565
Si1 O1 Si1 159.8(6) 19_665 .
O2 O2 Si1 74.7(3) 16_556 20
O2 O2 Si1 74.7(3) 16_556 .
Si1 O2 Si1 133.3(6) 20 .
O4 O3 Si1 60.9(5) . .
O4 O3 Si2 60.9(6) . 20
Si1 O3 Si2 115.3(7) . 20
O4 O3 V2 123.7(10) . .
Si1 O3 V2 134.4(6) . .
Si2 O3 V2 66.8(5) 20 .
O4 O3 V1 147.2(9) . .
Si1 O3 V1 136.6(5) . .
Si2 O3 V1 87.7(4) 20 .
V2 O3 V1 23.9(3) . .
O4 O3 Rb1 107.4(7) . .
Si1 O3 Rb1 117.4(5) . .
Si2 O3 Rb1 104.8(4) 20 .
V2 O3 Rb1 104.5(4) . .
V1 O3 Rb1 88.4(4) . .
O4 O3 Rb2 49.4(5) . .
Si1 O3 Rb2 110.2(5) . .
Si2 O3 Rb2 23.70(18) 20 .
V2 O3 Rb2 87.2(5) . .
V1 O3 Rb2 104.4(4) . .
Rb1 O3 Rb2 88.5(2) . .
O3 O4 Si1 75.7(6) . .
O3 O4 Si2 78.8(7) . 20
Si1 O4 Si2 141.0(6) . 20
O3 O4 O4 130.9(5) . 16_556
Si1 O4 O4 57.6(3) . 16_556
Si2 O4 O4 128.9(3) 20 16_556
O3 O4 Rb2 109.6(6) . .
Si1 O4 Rb2 173.3(6) . .
Si2 O4 Rb2 39.7(2) 20 .
O4 O4 Rb2 116.1(2) 16_556 .
O3 O4 Rb2 161.3(7) . 16_556
Si1 O4 Rb2 97.2(4) . 16_556
Si2 O4 Rb2 97.7(4) 20 16_556
O4 O4 Rb2 39.57(11) 16_556 16_556
Rb2 O4 Rb2 76.6(2) . 16_556
O3 O4 Rb1 54.1(6) . .
Si1 O4 Rb1 98.7(4) . .
Si2 O4 Rb1 89.5(4) 20 .
O4 O4 Rb1 140.97(11) 16_556 .
Rb2 O4 Rb1 87.9(2) . .
Rb2 O4 Rb1 144.6(2) 16_556 .
V2 O5 Si2 87.8(6) . 20
V2 O5 Si2 87.9(6) . .
Si2 O5 Si2 171.5(11) 20 .
V2 O5 V1 4.0(4) . .
Si2 O5 V1 87.6(6) 20 .
Si2 O5 V1 87.6(6) . .
V2 O5 Rb2 101.4(3) . 2
Si2 O5 Rb2 169.1(8) 20 2
Si2 O5 Rb2 18.9(3) . 2
V1 O5 Rb2 102.0(3) . 2
V2 O5 Rb2 101.4(3) . .
Si2 O5 Rb2 18.9(3) 20 .
Si2 O5 Rb2 169.1(8) . .
V1 O5 Rb2 102.0(3) . .
Rb2 O5 Rb2 150.3(5) 2 .
V2 O5 Rb2 38.8(6) . 15_556
Si2 O5 Rb2 90.6(6) 20 15_556
Si2 O5 Rb2 90.6(6) . 15_556
V1 O5 Rb2 42.8(3) . 15_556
Rb2 O5 Rb2 92.9(3) 2 15_556
Rb2 O5 Rb2 92.9(3) . 15_556
O6 O6 Si2 107.3(9) 9_556 .
O6 O6 V2 100.9(9) 9_556 15_556
Si2 O6 V2 135.2(5) . 15_556
O6 O6 Rb2 157.2(6) 9_556 2
Si2 O6 Rb2 54.9(3) . 2
V2 O6 Rb2 87.2(4) 15_556 2
O6 O6 V1 116.4(9) 9_556 15_556
Si2 O6 V1 133.9(5) . 15_556
V2 O6 V1 24.5(3) 15_556 15_556
Rb2 O6 V1 79.1(4) 2 15_556
O6 O6 Si2 42.4(6) 9_556 9_556
Si2 O6 Si2 134.9(6) . 9_556
V2 O6 Si2 58.7(4) 15_556 9_556
Rb2 O6 Si2 137.8(5) 2 9_556
V1 O6 Si2 77.6(3) 15_556 9_556
O6 O6 V2 50.1(7) 9_556 .
Si2 O6 V2 57.5(4) . .
V2 O6 V2 141.1(7) 15_556 .
Rb2 O6 V2 111.6(4) 2 .
V1 O6 V2 164.5(6) 15_556 .
Si2 O6 V2 87.1(4) 9_556 .
O6 O6 Rb1 78.67(18) 9_556 3_565
Si2 O6 Rb1 112.7(4) . 3_565
V2 O6 Rb1 106.3(4) 15_556 3_565
Rb2 O6 Rb1 119.8(5) 2 3_565
V1 O6 Rb1 90.2(4) 15_556 3_565
Si2 O6 Rb1 95.0(3) 9_556 3_565
V2 O6 Rb1 93.7(4) . 3_565
O6 O6 Rb2 14.1(4) 9_556 15_556
Si2 O6 Rb2 110.0(5) . 15_556
V2 O6 Rb2 90.2(5) 15_556 15_556
Rb2 O6 Rb2 149.1(5) 2 15_556
V1 O6 Rb2 109.1(4) 15_556 15_556
Si2 O6 Rb2 31.83(15) 9_556 15_556
V2 O6 Rb2 55.9(3) . 15_556
Rb1 O6 Rb2 90.5(2) 3_565 15_556
Rb2 O7 Si2 69.0(4) . 20
Rb2 O7 Si2 69.0(4) . 3
Si2 O7 Si2 128.4(6) 20 3
Rb2 O7 Rb2 112.6(7) . 16_556
Si2 O7 Rb2 111.4(4) 20 16_556
Si2 O7 Rb2 111.4(4) 3 16_556
V1 O8 V2 3.3(3) . .
V1 O8 Rb2 53.0(6) . 15_556
V2 O8 Rb2 56.3(4) . 15_556
V1 O8 Rb1 88.0(3) . .
V2 O8 Rb1 88.2(3) . .
Rb2 O8 Rb1 85.9(3) 15_556 .
V1 O8 Rb1 88.0(3) . 3_565
V2 O8 Rb1 88.2(3) . 3_565
Rb2 O8 Rb1 85.9(3) 15_556 3_565
Rb1 O8 Rb1 171.7(6) . 3_565
V2 O9 Si2 77.8(9) . 20
V2 O9 Si2 77.6(9) . .
Si2 O9 Si2 153(3) 20 .
V2 O9 V1 7.4(12) . .
Si2 O9 V1 78.6(9) 20 .
Si2 O9 V1 78.5(9) . .
V2 O9 Rb2 93.4(11) . .
Si2 O9 Rb2 19.0(12) 20 .
Si2 O9 Rb2 156(5) . .
V1 O9 Rb2 95.5(7) . .
V2 O9 Rb2 93.3(11) . 2
Si2 O9 Rb2 156(5) 20 2
Si2 O9 Rb2 19.0(12) . 2
V1 O9 Rb2 95.4(7) . 2
Rb2 O9 Rb2 146(4) . 2
Rb2 OW2 Rb2 75(2) 16_556 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Rb1 OW3 2.94(7) .
Rb1 OW3 2.94(7) 13_666
Rb1 O6 3.044(10) 8_666
Rb1 O6 3.044(10) 2_665
Rb1 O6 3.044(10) 20
Rb1 O6 3.044(10) 14_556
Rb1 O3 3.068(10) 13_666
Rb1 O3 3.068(10) .
Rb1 O3 3.068(10) 19_665
Rb1 O3 3.068(10) 7_556
Rb1 O8 3.3010(14) 13_666
Rb1 O8 3.3010(14) .
Rb2 O7 1.225(11) .
Rb2 Si2 1.652(3) 3
Rb2 Si2 1.652(3) 20
Rb2 O6 1.928(9) 3
Rb2 O6 1.928(9) 20
Rb2 V1 2.455(6) 14_556
Rb2 O4 2.536(7) 21
Rb2 O4 2.536(7) .
Rb2 V2 2.634(8) 14_556
Rb2 O8 3.058(18) 14_556
Rb2 O6 3.066(10) 7_556
Rb2 O6 3.066(10) 14_556
V1 V2 0.812(11) .
V1 O8 1.578(15) .
V1 O6 1.928(9) 9_556
V1 O6 1.928(9) 14_556
V1 O3 1.987(9) 20
V1 O3 1.987(9) .
V1 O5 2.168(17) .
V1 O9 2.42(3) .
V1 Rb2 2.455(6) 15_556
V1 Si2 2.640(5) .
V1 Si2 2.640(5) 20
V1 Rb1 3.609(2) 3_565
V2 O5 1.36(2) .
V2 O9 1.65(2) .
V2 O6 1.892(10) 14_556
V2 O6 1.892(10) 9_556
V2 O3 1.926(10) .
V2 O3 1.926(10) 20
V2 Si2 2.064(8) .
V2 Si2 2.064(8) 20
V2 O8 2.382(19) .
V2 O6 2.423(9) .
V2 O6 2.423(9) 20
Si1 O4 1.529(7) 16_556
Si1 O4 1.529(7) .
Si1 O1 1.592(2) .
Si1 O2 1.594(4) 16_556
Si1 O2 1.594(4) .
Si1 O3 1.695(8) 16_556
Si1 O3 1.695(8) .
Si1 Rb2 4.059(2) 16_556
Si1 Rb1 4.1308(9) 4_664
Si2 O6 1.601(8) .
Si2 O5 1.601(3) .
Si2 O4 1.623(7) 20
Si2 O7 1.632(5) 2
Si2 O9 1.645(12) .
Si2 Rb2 1.652(3) 2
Si2 O3 1.822(12) 20
Si2 O6 2.265(10) 9_556
Si2 Rb2 3.914(3) 15_556
Si2 Rb1 3.948(3) 3_565
O1 Si1 1.592(2) 19_665
O2 O2 0.843(19) 16_556
O2 Si1 1.594(4) 20
O3 O4 1.201(13) .
O3 Si2 1.822(12) 20
O4 Si2 1.623(7) 20
O4 O4 1.638(17) 16_556
O4 Rb2 3.575(9) 16_556
O5 Si2 1.601(3) 20
O5 Rb2 3.083(4) 2
O5 Rb2 3.554(17) 15_556
O6 O6 1.196(19) 9_556
O6 V2 1.892(10) 15_556
O6 Rb2 1.928(9) 2
O6 V1 1.928(9) 15_556
O6 Si2 2.265(10) 9_556
O6 Rb1 3.044(9) 3_565
O6 Rb2 3.066(10) 15_556
O7 Si2 1.632(5) 20
O7 Si2 1.632(5) 3
O7 Rb2 3.233(11) 16_556
O8 Rb2 3.058(18) 15_556
O8 Rb1 3.3010(13) 3_565
O9 Si2 1.640(12) 20
O9 Rb2 3.12(3) 2
OW2 Rb2 3.19(8) 16_556
